Article Poisoning Eﬀects of Phosphorus, Potassium and Lead on V2O5-WO3/TiO2 Catalysts for Selective Catalytic Reduction with NH3
Jifa Miao 1,2,3, Xianfang Yi 1,2,3, Qingfa Su 1,2,3, Huirong Li 1,2,3, Jinsheng Chen 1,2,* and Jinxiu Wang 1,2,*
1 Center for Excellence in Regional Atmospheric Environment, Institute of Urban Environment, Chinese Academy of Sciences, Xiamen 361021, China; [email protected] (J.M.); [email protected] (X.Y.); [email protected] (Q.S.); [email protected] (H.L.) 2 Key Laboratory of Urban Environment and Health, Institute of Urban Environment, Chinese Academy of Sciences, Xiamen 361021, China 3 University of Chinese Academy of Sciences, Beijing 100049, China * Correspondence: [email protected] (J.C.); [email protected] (J.W.); Tel./Fax: +86-592-6190765 (J.C.); +86-592-6190548 (J.W.) Received: 13 February 2020; Accepted: 17 March 2020; Published: 20 March 2020
Abstract: The poisoning eﬀect of single elements on commercial V2O5-WO3/TiO2 catalysts has been studied in the past decades. In this study, the combined eﬀects of two multi-element systems (phosphorus-potassium and phosphorus-lead) on V2O5-WO3/TiO2 catalysts were studied by diverse characterizations. The results show that potassium and lead can result in the deactivation of catalysts to diﬀerent degrees by reacting with active acid sites and reducing the amount of V5+. However, phosphorus displays slight negative inﬂuence on the NOx conversion of the catalyst due to the comprehensive eﬀect of reducing V5+ amount and generating new acid sites. The samples poisoned by phosphorus–potassium and phosphorus–lead have higher NOx conversion than that by potassium or lead, because doped potassium or lead atoms may react with new acid sites generated by phosphate, which liberates more V–OH on the surface of catalysts and reduces the poisoning eﬀects of potassium or lead on vanadium species and active oxygen species.
Keywords: commercial SCR catalysts; multi-element poisoning; phosphorus; lead; potassium; combined eﬀect
The selective catalytic reduction (SCR) of nitrogen oxides (NOx) with ammonia is one of the most eﬀective technologies to reduce NOx emission generated by combustion process [1–3], such as coal-ﬁred power plants and municipal solid waste incinerators . The catalyst mostly used for this purpose is V2O5-WO3/TiO2.V2O5 is considered as the active phase and WO3 is considered as a promoter that inhibits the transformation of anatase to rutile, favors the spreading of the vanadia on the catalyst surface, and increases the acidity of the catalyst [5,6]. Though V2O5-WO3/TiO2 catalysts show excellent activity in NH3-SCR process, many compounds including alkali/alkali earth metal elements, Pb, Zn, P and As are found in exhaust ﬂue gas streams, which can lead to the deactivation of SCR catalysts in their lifetime. The deactivation mechanism of single element was studied in the past decades [1,7–13]. Recently, the combined eﬀects of diﬀerent elements in the ﬂue gas aroused the attention of scholars. Yu et al. [14,15] suggested that SO2 in the ﬂue gas promoted the activity of K- and Pb-poisoned catalysts. Kong et al.  discovered that new acid sites generated on the SCR catalyst by loading HgCl2. Our recent work indicated SO2 and HCl can
Catalysts 2020, 10, 345; doi:10.3390/catal10030345 www.mdpi.com/journal/catalysts Catalysts 2020, 10, 345 2 of 14 promote the activity of Pb-poisoned SCR catalyst . However, few studies were about the combined eﬀects of P and other poisoning elements. Schobing et al.  found the simultaneous presence of Ca and Zn on the catalyst increased the deactivation, but the additivity of individual eﬀects was not observed and the presence of phosphates anions reduced the poisoning eﬀects of Ca and Zn. Klimczak et al.  found an alleviated poisoning of Ca in the presence of phosphates and sulfates due to a regeneration of the ammonia adsorption capacity of the catalyst. It seems that phosphorus (P) could neutralize the negative eﬀects of some poisoning elements, even though P has relatively small negative inﬂuence on V2O5-WO3/TiO2 catalysts in consideration of the large amount of phosphorus addition. However, Chen et al.  discovered that alkali metal had the strongest poisoning eﬀect on the V-based catalyst, and the poisoning eﬀect of Pb was between K2O and Na2O (K2O > PbO > Na2O). And K is a major component of alkali metals in the coal-ﬁred ﬂue gas. Tokarz et al.  measured a large amount of Pb contained in the ﬂue gas of municipal solid waste incinerators. It is; therefore, desirable to study the combined poisoning eﬀects of P and K or Pb on commercial V2O5-WO3/TiO2 catalysts. In this work, the commercial V2O5-WO3/TiO2 catalyst was deactivated by P, K, Pb and the combination of P and K or Pb. The combined poisoning eﬀects of P and K or Pb were studied by a series of characterizations. The inﬂuence of surface O, V, P and Ti species was investigated by X-ray photoelectron spectroscopy (XPS) and the amount and types of acid sites present in catalysts were further studied by temperature-programmed desorption of NH3 (NH3-TPD) and in situ diﬀuse reﬂectance infrared Fourier-transform spectroscopy (in situ DRIFTS).
2. Results and Discussion
2.1. Catalytic Activity Figure1a shows the SCR activity of the catalyst samples in the temperature range of 250 to 1 380 ◦C under a GHSV of 60,000 h− . The experiments at each speciﬁc temperature were maintained for 1 h. The NOx conversion of fresh sample keeps around 90% in the temperature range of 250 to 380 ◦C. Compared with fresh sample, the NOx conversion of D-P (poisoned by P) decreases slightly (~4%). The poisoning eﬀects of K and Pb on the V2O5-WO3/TiO2 catalyst obviously decrease the NOx conversion of D-K (poisoned by K) and D-Pb (poisoned by Pb) sample. However, the NOx conversion rates of D-P-K (poisoned by P and K) and D-P-Pb (poisoned by P and Pb) pretreated with (NH4)2HPO4 are higher than that of D-K and D-Pb, respectively. It implies that the treatment with (NH4)2HPO4 counteracts the poisoning eﬀects of K and Pb on the catalyst to some degree. Furthermore, Figure S1a shows the N2 selectivity of poisoned catalyst increases at increasing temperature in the range 250–280 ◦C. Then N2 selectivity of poisoned catalyst decreases with increasing temperature above 300 ◦C. Figure1b shows the NO x conversion of the fresh catalyst and poisoned samples at 350 ◦C for 3500 min. The fresh catalyst shows high stability. Its NOx conversion reaches the stable stage in 10 min and keeps around 95% until the end of the test. The NOxconversion rates of D-K and D-Pb samples also slightly decrease with time. The NOx conversion rates of the catalysts treated by (NH4)2HPO4 (D-P, D-P-K and D-P-Pb) decrease by 2%, 3% and 3%, respectively, in the ﬁrst 1500 min, and then are relatively stable during the test. The N2 selectivity of fresh sample keeps stable, and that of the poisoned catalyst decreases a little during the test (Figure S1b).
2.2. Structure and Surface Acid Sites
XRD patterns of fresh catalyst and poisoned samples are displayed in Figure2. The 2 θ = 25.30◦, 36.95◦, 37.79◦, 38.57◦, 48.04◦, 53.89◦, 55.06◦, 62.11◦, 62.69◦, 68.76◦, 70.29◦, 74.05◦ and 76.03◦ diﬀraction peaks correspond to tetragonal anatase phase of titanium dioxide (PDF card-03-065-5714). Only anatase phase TiO2 is observed in all samples and it indicates that the dopants do not change the crystal type of TiO2. In addition, it also suggests the ﬁnely dispersed or amorphous V2O5 and other dopants on the Catalysts 2020, 10, 345 3 of 14
surface of TiO2. The SEM-EDS images of V and W evidence the presence of W, V and the dopants on the catalyst surface (Figure S2).
Figure 1. (a) NOx conversion of fresh catalyst and poisoned catalyst. (b) NOx conversion of fresh catalyst and poisoned catalyst at 350 ◦C with time. Reaction conditions: [NO] = [NH3] = 500 ppm, 1 [O2] = 5 vol. %, total ﬂow rate = 1.2 L/min, GHSV = 60,000 h− .
Figure 2. XRD patterns of fresh and poisoned catalysts. Catalysts 2020, 10, 345 4 of 14
Table1 summarizes the element loading amount, speciﬁc surface areas (S BET), total pore volume (Vp) and average pore diameter (DA) for all catalysts. The N2 adsorption-desorption isotherms of all samples and pore size distribution are displayed in Figures S3 and S4. According to the International Union of Pure and Applied Chemistry (IUPAC) classiﬁcation, the isotherms are type-IV nitrogen isotherm corresponding to typical mesoporous materials. The SBET and Vp of the D-Pb and D-K samples are almost similar to the fresh catalyst, suggesting that Pb and K have little inﬂuence on the pore structure of the catalyst. The treatment with (NH4)2HPO4 decreases the SBET and increases the DA of the samples, The SEM images of fresh catalysts and poisoned samples are exhibited in Figure S5. A little agglomeration is observed on the samples containing P, which may block the pores and change SBET and Vp of the samples.
Table 1. Element loading amount, speciﬁc surface areas, total pore volume and average pore diameter of samples.
Loading Amount (wt %) 2 3 Sample SBET (m /g) VP* (cm /g) DA (nm) P K Pb Fresh - - - 41.8 0.231 11.06 D-P 0.95 - - 34.3 0.207 12.09 D-Pb - - 0.86 41.6 0.227 10.74 D-K - 0.48 - 41.5 0.234 12.75 D-P-K 0.91 0.45 - 31.3 0.225 14.38 D-P-Pb 0.88 - 0.87 34.9 0.215 12.34
*VP is obtained at the relative pressure of P/P0 = 0.99; - denotes it is not detected by SEM-EDS.
The results of structure analysis imply that signiﬁcant deactivation eﬀect of Pb and K may well result from the chemical reaction between poisoning elements and active sites over catalysts. Moreover, the NOx conversion of samples containing P and another poisoning element is not aﬀected by the reduced SBET. There may be other reasons for the activity change of these samples. Therefore, further characterizations were conducted. It has been recognized that the surface acid sites over V2O5-WO3/TiO2 catalyst play a crucial role in the selective catalytic reduction process [4,20]. Therefore, the NH3-TPD was performed to investigate the combined eﬀects of poison elements on acid sites of the catalyst. The NH3-TPD proﬁle are exhibited in Figure3. It shows that all curves recorded from 100–600 ◦C are divided into two parts. The part below 280 ◦C is attributed to NH3 desorption on the weak acid sites, and the other part above 280 ◦C is ascribed to NH3 desorption on the strong acid sites. The total amounts of NH3 adsorption on each sample are calculated from the integrated areas of the corresponding curves and normalized by the value of Fresh sample. They are sequenced as follows: D-P (1.27) > fresh (1.00) > D-P-Pb (0.68) > D-Pb (0.64) > D-P-K (0.60) > D-K (0.23). It shows that the amount of desorbed NH3 on the D-P sample increases by 27% compared with fresh sample especially the amount of NH3 adsorbed on the weak acid sites. However, the Mass Spectrum (MS) signal of desorbed NH3 decreases obviously with doping K (by 77%) or Pb (by 36%), which suggests the doping of K or Pb reduces the acidity of catalyst signiﬁcantly. The treatment with (NH4)2HPO4 increases the amount of NH3 adsorption of K and Pb poisoning samples by 161% and 6%, respectively. It may be the reason that D-P-K and D-P-Pb samples have higher DeNOx eﬃciency than D-K and D-Pb samples. Besides the surface concentration of acid sites, the types of acid sites are also important for the SCR catalysts . Therefore, a set of in situ DRIFTS experiments was conducted to obtain a thorough understanding of the interaction between NH3 and the surface acid sites. The in situ DRIFTS results of samples exposed to 500 ppm NH3 in N2 at 350 and 200 ◦C for 30 min 1 are displayed in Figure4. Figure4a shows that three bands at 1605, 1401 and 1238 cm − are detected in 1 the Fresh catalyst at 350 ◦C. It is recognized that the bands located at 1605 and 1238 cm− are ascribed 1 to NH3 adsorbed on Lewis acid sites [21–24], and the band at 1401 cm− is associated with asymmetric Catalysts 2020, 10, 345 5 of 14 deformation modes of ammonium ions on Brønsted acid sites [25,26]. The observed bands at 1610, 1 1426, 1409 and 1659 cm− on D-P sample are stronger obviously than that on fresh sample at 350 ◦C. 1 The band located at 1659, 1426 and 1409 cm− were proved to be NH3 adsorbed on the Brønsted acid sites [23,27,28]. It implies that the treatment with (NH4)2HPO4 generates new Brønsted and Lewis acid sites and improves the acidity of V2O5-WO3/TiO2 catalyst [29–31]. For the in situ DRIFTS spectrum of D-K and D-Pb, only very weak bands are detected. It indicates that K and Pb can result in huge damage to Lewis acid sites and Brønsted acid sites. However, when K or Pb is introduced to the sample pretreated with (NH4)2HPO4, the bands attributed to NH3 adsorbed on Lewis acid sites and Brønsted acid sites can be detected with enhanced intensity. It suggests the treatment with (NH4)2HPO4 can weaken the poisoning eﬀects of K and Pb on the V2O5-WO3/TiO2 catalyst.
Figure 3. NH3-TPD proﬁles of fresh and poisoned catalyst samples.
Figure 4. In situ DRIFTS spectra of NH3 adsorption on fresh and poisoned catalysts at 350 ◦C(a) and 200 ◦C(b) for 30 min. Catalysts 2020, 10, 345 6 of 14
The stability of the adsorbed ammonia on the catalysts was analyzed by comparing the spectra of samples collected at 200 and 350 ◦C, respectively. The intensity of all peaks due to the adsorbed ammonia decreased with increasing temperature except the peaks detected on D-P. As shown in 1 Figure4b, the bands located at 1662, 1608, 1445, 1298 and 1238 cm − are observed on the fresh catalysts. 1 + The bands at 1662 and 1445 cm− are assigned to NH4 chemisorbed on Brønsted acid site. The bands 1 at 1608, 1298 and 1238 cm− are attributed to NH3 adsorbed on the Lewis acid sites [21,32,33]. When the temperature reaches 350 ◦C, the bands on the fresh catalysts become to weaken and the band at 1 1298 cm− vanishes. However, the bands on the D-P samples still keep strong intensity especially the 1 bands at 1426 and 1409 cm− . It implies that the acid sites generated by P species have higher thermo stability. This is maybe the reason the D-P has good NOx conversion at high temperature. The Brønsted acid sites on the D-P-K and D-P-Pb decrease with increasing temperature clearly. The doped K and Pb atoms tend to react with acid sites generated by P species. The results suggest that the treatment with (NH4)2HPO4 can weaken the poisoning eﬀect of Pb and K on fresh catalyst because of the formation of new Lewis acid sites and Brønsted acid sites. A total of 500 ppm NO and 5% O2 were introduced to the D-P sample and fresh sample pretreated with NH3 and purged with N2 for 10 min. The reaction spectra between NO + O2 and adsorbed 1 NH3 species are presented in Figure5. For the spectrum of fresh catalyst, the band at 1238 cm − gradually weakens with time and vanishes after NO + O2 is introduced for 30 min, and the bands 1 at 1605 and 1401 cm− weaken during the test. In addition, new bands are detected at 1626 and 1 1599 cm− , which could be assigned to adsorbed NO2 and bridged nitrate [34,35]. The results indicate that adsorbed NH3 species on fresh sample are consumed in the NO + O2 stream. For the spectrum 1 of D-P sample, the bands at 1659, 1607, 1426 and 1409 cm− weaken during test time and the band 1 1 at 1659 cm− almost vanishes for 30 min. A new band located at 1595 cm− assigned to adsorbed bridged nitrate is detected. The results indicate that adsorbed NH3 species on Lewis acid sites and Brønsted acid sites, partly generated by the treatment of (NH4)2HPO4, can be consumed in the NO + O2 stream as well. The above experiments suggest that the reaction mechanism on the samples pretreated with (NH4)2HPO4 still follows the Eley–Rideal mechanism: Adsorbed ammonia species react with gas-phase or weakly-adsorbed NO .
2.3. Surface Chemical State XPS was carried out to illustrate the change of oxidation state of the active species after poisoning. Figure6 shows the XPS results of O 1s, V 2p 3/2, P 2p and Ti 2p. The spectra of O 1s were ﬁtted into three peaks which are the lattice oxygen in the metal oxides (Oγ), the surface oxygen by hydroxyl species (Oβ) and the absorbed oxygen or/and weakly bonded oxygen species (Oα)[21,37,38]. The positions and concentrations of oxygen species are displayed in the Table2. Surface chemisorbed oxygen has been reported to be the most active oxygen and plays an important role in oxidation reactions [20,39]. It can be found that Oβ concentration of D-P sample is higher than that of fresh sample, indicating that there are more hydroxyl species (–OH) after doping which can form P–OH on the surface of catalysts . However, the D-P sample has lower NOx conversion than fresh catalyst, indicating P-OH has lower activity than that of V–OH. The Oβ concentration of D-K and D-Pb samples is lower than that of fresh sample, suggesting K and Pb can react with surface hydroxyl species and form –O–K or –O–Pb–O–, in accordance with other researches [20,40]. For D-P-K and D-P-Pb samples, it can be found that Oβ concentration increases largely, suggesting more –OH species still exist on the catalyst surface. The binding energy value of Oγ shifts from 529.9 to 529.7 and 529.8 eV after the Pb and K doping. This may be because Pb and K donates electrons to lattice oxygen. However, in the D-P-K and D-P-Pb samples, the binding energy value of Oγ keeps similar to the fresh catalyst. It suggests that the treatment with (NH4)2HPO4 may obstruct the electron interaction of Pb and K and the catalyst. Catalysts 2020, 10, 345 7 of 14
Figure 5. In situ DRIFTS spectra of the reaction between NO + O2 and adsorbed NH3 species over (a) fresh and (b) D-P at 350 ◦C.
Table 2. The position and atom ratio of O spices in XPS spectra for each sample.
Samples Oα %Oβ %Oγ % Fresh 532.4 (18.1) 531.3 (17.4) 529.9 (64.5) D-P 532.3 (19.3) 531.2 (25.4) 529.9 (55.3) D-Pb 532.3 (22.1) 531.0 (14.6) 529.7 (63.3) D-K 532.3 (22.9) 531.0 (5.7) 529.8 (71.4) D-P-Pb 532.4 (22.8) 531.4 (22.8) 529.9 (54.4) D-P-K 532.3 (26.2) 531.3 (17.9) 530.0 (55.9)
Based on previous reports [41,42], the SCR activity of catalyst is positively correlated with the 5+ 4+ 5+ surface V /V ratio. The spectra of V 2p3/2 are ﬁtted into two peaks related to V (~ 517.1 eV) and V4+ (~ 516.2 eV) . The atomic ratio of V5+/V4+ can be determined according to the peaks area ratio of V5+/V4+. Table3 summarizes the peak position and atomic ratio of V 5+/V4+ in diﬀerent samples. The atomic ratio of V5+/V4+ decreases obviously after doping poisoning elements, indicating P, Pb 5+ 4+ and K can result in the transformation from V into V in V2O5-WO3/TiO2 catalysts. However, the adverse inﬂuence of P on surface V5+/V4+ ratio was much weaker than K and Pb. The atomic ratio of V5+/V4+ decreases from 1.21 to 0.43 and 0.51 after doping with K and Pb. Compared with D-K and D-Pb, the atomic ratio of V5+/V4+ in D-P-K and D-P-Pb samples increases largely. The result indicates 5+ 4+ that the treatment with (NH4)2HPO4 can inhibit the transformation from V into V resulting from the adverse inﬂuence of Pb and K. Catalysts 2020, 10, 345 8 of 14
The P 2p binding energy of samples containing P is detected at 133.8 eV, suggesting that P in the samples exists in a pentavalent-oxidation state (P5+), and no peak is observed at 128.6 eV that is the characteristic binding energy of P 2p in Ti-P, indicating the absence of Ti-P bonds in the samples [29,30,45].
5+ 4+ Table 3. XPS results of V 2p3/2 and surface atomic ratio of V /V for each sample.
Binding Energy (eV) Samples V5+/V4+ V4+ V5+ Fresh 516.1 517.1 1.21 D-P 516.2 517.1 0.86 D-Pb 516.1 517.1 0.51 D-K 516.2 517.1 0.43 D-P-K 516.2 517.1 0.71 D-P-Pb 516.3 517.2 0.83
Figure 6. Cont. Catalysts 2020, 10, 345 9 of 14
Figure 6. XPS spectra of the O 1s, V 2p3/2, P 2p and Ti 2p of fresh and poisoned samples.
For the spectra of Ti 2p, two peaks centered at 458.6–459 eV and 464.4–464.9 eV can be ascribed 4+ to Ti 2p3/2 and Ti 2p1/2, respectively, suggesting the presence of Ti in all samples [25,46]. When the catalyst treated with (NH4)2HPO4, the Ti 2p3/2 and Ti 2p1/2 peaks shift to higher energies, from 458.7 to 458.9 eV and 464.6 to 464.8 eV, respectively. It means the titanium species in D-P samples have lower density of electron cloud density than that in fresh samples [45,47]. It may because the electrons around the titanium species transfer to oxygen species, which interact with P dopants. It also proves 5+ 4+ that P can replace part of Ti in TiO2 lattice to form a Ti–O–P linkage. The similar location of the Ti 2p peaks for fresh, D-K and D-Pb samples, indicates that K and Pb may not react with TiO2 [4,48]. In addition, D-P-K and D-P-Pb have a similar Ti 2p peak center with D-P, which implies that K or Pb does not aﬀect the reaction between P species and TiO2. The XPS spectra of W 4f were displayed in the Figure S6 and the information was supplied in the Supplementary Materials.
2.4. Poisoning Eﬀect of Phosphorus, Potassium and Lead on V2O5-WO3/TiO2 Catalysts
Based on the NH3-TPD, DRIFT, XPS spectra analysis and previous studies [29,49,50], the proposed combined poisoning eﬀect of phosphorus, potassium or lead on V2O5-WO3/TiO2 can be concluded in + Figure7. For fresh catalyst, based on Eley–Rideal mechanism, the adsorbed NH 4 species on –OH can be activated by V5+ active sites and react with NO in the ﬂue gas [51,52]. The poisoning eﬀects of K and Pb on the catalyst can be assigned to the neutralization of the acid sites, the decrease of surface 5+ chemisorption oxygen and the reduction of V species [10,40]. This results in weakening the NH3 adsorption capacity and reducibility of the catalyst. After the treatment with (NH4)2HPO4, the doped P species occupy the acid sites. However, new Brønsted acid sites (P–OH) form , and the acid sites Catalysts 2020, 10, 345 10 of 14
+ also have the ability to adsorb NH3. The NH4 species adsorbed on the Brønsted acid sites (P–OH) could be activated by surface V active sites due to the excellent redox property of nearby V5+ species. Hence, the slightly weakened NH3-SCR performance of D-P samples can be assigned to the reduction of V5+ species. For D-P-K and D-P-Pb, the in situ DRIFTS analysis results suggest doped Pb and K atoms may react with acid sites generated by phosphate, and make them inactive in the adsorption of NH3. Each K atom consumes one acid site, and each Pb atom reacts with two acid sites. Hence, it seems that more K and Pb around the P atom will liberate more V–OH on the surface of catalysts, so the treatment with (NH4)2HPO4 alleviates the poisoning eﬀect of potassium or lead on the catalysts .
Figure 7. Schematic diagram of the combined eﬀect of phosphorus, potassium and or lead on
3. Materials and Methods
3.1. Catalysts Preparation
The commercial V2O5-WO3/TiO2 catalyst (named as Fresh, with 1.16 wt.% V and 2.42 wt.% W) was ground and sieved to 60–80 mesh. All the chemicals used in the catalyst preparation process were analytical grade and purchased from Sinopharm Chemical Reagent Co., Ltd (Shanghai, China). The P poisoned samples were prepared by impregnating the commercial catalyst particles into aqueous (NH4)2HPO4 (0.25 mol/L) solution for 6 h at room temperature. Then the samples were dried at 105 ◦C for 12 h followed by calcination at 500 ◦C for 4 h in a muﬄe furnace. The P poisoned catalyst was denoted as D-P. Fresh catalysts and D-P sample were impregnated into aqueous KNO3 (0.13 mol/L) or Pb(NO3)2 (0.25 mol/L) solution for 6 h at room temperature. Then the samples were dried at 105 ◦C for 12 h followed by calcination at 500 ◦C for 4 h in a muﬄe furnace. The samples were denoted as D-K, D-Pb, D-P-K and D-P-Pb. The element loading amount detected by SEM-EDS is summarized in Table1.
3.2. Activity Test The catalytic activities of the samples were evaluated in a simulated ﬁxed-bed reactor made of quartz tube with the dimensions of Φ 6.2 580 mm in the laboratory. The simulated ﬂue gas consisted × of 500 ppm NO, 500 ppm NH3, 5% O2 and N2 balance. In each experimental run, the catalysts loaded Catalysts 2020, 10, 345 11 of 14
3 1 in the reactor were 1.2 cm and the gas hourly space velocity (GHSV) was kept at 60,000 h− . For this system, the concentrations of NO, NO2 and NH3 were measured by an Antaris IGS analyzer (Thermo Fisher Company, Waltham, M.A., USA) and the concentration of O2 was measured by a ﬂue gas analyzer (T-350, Testo Company, Hampshire, United Kingdom). The conversion of NOx was deﬁned as:
CNO ,in CNO ,out NOx conversion = x − x 100% CNOx,in ×
2CN2O,out N2 selectivity = 1 100% −C + C C CNH out × NOx,in NH3,in − NOx,out − 3, where CNOx,in and CNOx,out are the NOx concentration (NO + NO2) of the simulated gas stream in the inlet and outlet of the reactor, CNH3,in and CNH3,out are the inlet and outlet concentrations of NH3, and
CN2O,out is the outlet concentration of N2O.
3.3. Catalysts Characterization The morphology and elemental analysis of samples was conducted by scanning electron microscope-energy dispersive X-ray spectrometer (SEM-EDS, S-4800, Hitachi, Tokyo, and 51-ADD0009, Horiba, Tokyo; Japan) and X-ray ﬂuorescence spectrometer (XRF, Axios mAX, PANalytical B.V., Almelo, Netherlands) equipped with a Rh-anode X-ray tube. The Brunauer–Emmett–Teller (BET) speciﬁc surface area and porosities of the samples were measured on a NOVA 1200e surface area and pore size analyzer (Quantachrome, Boynton Beach, F.L., USA) at 77 K. X-ray diﬀraction (XRD) patterns were recorded on X Pert Pro XRD diﬀractometer (PANalytical B.V., Almelo, Netherlands) with Cu Kα radiation (40 kV, 40 mA). The temperature-programmed desorption of ammonia (NH3-TPD) on samples was carried out on a chemisorption analyzer (ChemBET-3000TPR-TPD, Quantachrome, Boynton Beach, F.L., USA)-mass spectrum (DYCOR LC-D200, Ametek, Kent, O.H., USA). A total of 100 mg of the sample was treated in helium at 500 ◦C for 1 h and cooled to room temperature. Then the sample was exposed to 5% NH3 for 40 min and subsequently purged with helium at 100 ◦C for 30 min to remove weakly-adsorbed NH3 from the surface. Finally, the sample was heated to 600 ◦C at a rate of 10 ◦C/min in He and the signal of NH3 was recorded by mass spectrum. In situ diﬀuse reﬂectance infrared Fourier-transform spectra (DRIFTS) were collected using a Bruker Vertex70 infrared spectrometer (Billerica, M.A., USA) with KBr optics and a mercury-cadmium-telluride (MCT) detector. The sample was treated at 500 ◦C for 1 h and then cooled to the desired temperature in N2 atmosphere. The spectra were collected with 500 ppm NH3 in N2 at the set time. All the spectra 1 were collected at a resolution of 4 cm− by accumulating 64 scans. The spectra obtained in this study were transformed into absorption spectra by using Kubelka–Munk function. X-ray photoelectron spectra (XPS) were measured with a Thermo ESCALAB 250 (Waltham, M.A., USA) using monochromated Al Kα X-rays (h = 1486.6 eV) as a radiation source at 150 W. Sample charging eﬀects were eliminated by correcting the observed spectra with the C 1s binding energy (BE) value of 284.6 eV. The analysis of XPS spectra of samples was conducted by “Avantage” software supplied by Thermo Fisher Scientiﬁc Corporation, and uses “Scoﬁeld factor” as sensitive factor.
In this study, P, K and Pb decrease the DeNOx eﬃciency of commercial V2O5-WO3/TiO2 catalysts to diﬀerent degrees. Furthermore, the doping of P, K and Pb does not change crystalline phase and textural structure of commercial catalysts. However, the treatment with (NH4)2HPO4 improves the NOx conversion of Pb- and K-poisoned catalysts. That may be because the samples pretreated with (NH4)2HPO4 have higher content of acid sites with higher thermal stability. Moreover, they have increased V5+/V4+ ratio and active oxygen species, including V-OH and P-OH, on the surface of Catalysts 2020, 10, 345 12 of 14
catalysts. It is believed that the treatment with (NH4)2HPO4 can decrease the poisoning eﬀects of K and Pb on commercial V2O5-WO3/TiO2 catalysts. This work may oﬀer the reference to further research in the complex poisoning eﬀects of multiple elements on commercial V2O5-WO3/TiO2 catalysts.
Supplementary Materials: The following are available online at http://www.mdpi.com/2073-4344/10/3/345/s1, Figure S1: (a) The N2 selectivity of fresh and poisoned samples; (b) the N2 selectivity of fresh and poisoned samples at 350 ◦C with time, Figure S2: The SEM-EDS images of fresh and poisoned catalyst, Figure S3: N2 adsorption-desorption isotherm of fresh and poisoned samples, Figure S4: The pore size distribution of fresh and poisoned samples, Figure S5: The SEM images of fresh catalysts and poisoned samples, Figure S6: XPS spectra of the W 4f of fresh and poisoned samples. Author Contributions: Conceptualization, J.M., J.W. and J.C.; Data curation, J.W.; Investigation, J.M., X.Y. and Q.S.; Supervision, J.C. and J.W.; Writing—original draft, J.M.; Writing—review and editing, J.C. and J.W. All authors have read and agree to the published version of the manuscript. Funding: This work is ﬁnancially supported by Youth Innovation Promotion Association, Chinese Academy of Sciences (2020309), the Strategic Priority Research Program of the Chinese Academy of Sciences (XDB05050500), Bureau of Science and Technology, Fujian Province, China (2015H0043) and Fujian Institute of Innovation, Chinese Academy of Sciences. Acknowledgments: The authors are grateful to the tests oﬀered by the Analysis and Testing Center, Institute of Urban Environment, Chinese Academy of Sciences, Xiamen. Conﬂicts of Interest: The authors declare no conﬂicts of interest.
1. Schobing, J.; Tschamber, V.; Brilhac, J.F.; Auclaire, A.; Vonarb, R. Investigation of the impact of calcium, zinc and phosphorus on DeNOx activity of a commercial SCR catalyst. Top. Catal. 2016, 59, 1013–1019. [CrossRef] 2. Peng, Y.; Li, J.; Si, W.; Luo, J.; Wang, Y.; Fu, J.; Li, X.; Crittenden, J.; Hao, J. Deactivation and regeneration of a commercial SCR catalyst: Comparison with alkali metals and arsenic. Appl. Catal. B Environ. 2015, 168, 195–202. [CrossRef] 3. Putluru, S.S.R.; Schill, L.; Gardini, D.; Mossin, S.; Wagner, J.B.; Jensen, A.D.; Fehrmann, R. Superior DeNOx activity of V2O5–WO3/TiO2 catalysts prepared by deposition–precipitation method. J. Mater. Sci. 2014, 49, 2705–2713. [CrossRef]
4. Miao, J.; Li, H.; Su, Q.; Yu, Y.; Chen, Y.; Chen, J.; Wang, J. The combined promotive eﬀect of SO2 and HCl on Pb-poisoned commercial NH3-SCR V2O5-WO3/TiO2 catalysts. Catal. Commun. 2019, 125, 118–122. [CrossRef] 5. Nicosia, D.; Elsener, M.; Kröcher, O.; Jansohn, P. Basic investigation of the chemical deactivation of
V2O5/WO3-TiO2 SCR catalysts by potassium, calcium, and phosphate. Top. Catal. 2007, 42, 333–336. [CrossRef] 6. Madia, G.; Elsener, M.; Koebel, M.; Raimondi, F.; Wokaun, A. Thermal stability of vanadia-tungsta-titania catalysts in the SCR process. Appl. Catal. B Environ. 2002, 39, 181–190. [CrossRef] 7. Kling, Å.; Andersson, C.; Myringer, Å.; Eskilsson, D.; Järås, S.G. Alkali deactivation of high-dust SCR catalysts used for NOx reduction exposed to ﬂue gas from 100 MW-scale biofuel and peat ﬁred boilers: Inﬂuence of ﬂue gas composition. Appl. Catal. B Environ. 2007, 69, 240–251. [CrossRef] 8. Khodayari, R.; Odenbrand, C.U.I. Deactivating eﬀects of lead on the selective catalytic reduction of nitric
oxide with ammonia over a V2O5/WO3/TiO2 catalyst for waste incineration applications. Ind. Eng. Chem. Res. 1998, 37, 1196–1202. [CrossRef] 9. Hu, W.; Gao, X.; Deng, Y.; Qu, R.; Zheng, C.; Zhu, X.; Cen, K. Deactivation mechanism of arsenic and resistance 2- eﬀect of SO4 on commercial catalysts for selective catalytic reduction of NOx with NH3. Chem. Eng. J. 2016, 293, 118–128. [CrossRef]
10. Chen, J.P.; Yang, R.T. Mechanism of poisoning of the V2O5/TiO2 catalyst for the reduction of NO by NH3. J. Catal. 1990, 125, 411–420. [CrossRef]
11. Hiroyuki, K.; Katsumi, T.; Odenbrand, C.U.I. The role of K2O in the selective reduction of NO with NH3 over a V2O5(WO3)-TiO2 commercial selective catalytic reduction catalyst. J. Mol. Catal. A Chem. 1999, 139, 189–198. 12. Larsson, A.C.; Einvall, J.; Sanati, M. Deactivation of SCR catalysts by exposure to aerosol particles of potassium and zinc salts. Aerosol Sci. Technol. 2007, 41, 369–379. [CrossRef] Catalysts 2020, 10, 345 13 of 14
13. Odenbrand, C.U.I. CaSO4 deactivated V2O5-WO3/TiO2 SCR catalyst for a diesel power plant. Characterization and simulation of the kinetics of the SCR reactions. Appl. Catal. B Environ. 2018, 234, 365–377. [CrossRef]
14. Yu, Y.; Wang, J.; Chen, J.; Meng, X.; Chen, Y.; Chi, H. Promotive eﬀect of SO2 on the activity of a deactivated commercial selective catalytic reduction catalyst: An in situ DRIFT study. Ind. Eng. Chem. Res. 2014, 53, 16229–16234. [CrossRef]
15. Yu, Y.; Miao, J.; He, C.; Chen, J.; Li, C.; Douthwaite, M. The remarkable promotional eﬀect of SO2 on Pb-poisoned V2O5-WO3/TiO2 catalysts: An in-depth experimental and theoretical study. Chem. Eng. J. 2018, 338, 191–201. [CrossRef] 16. Kong, M.; Liu, Q.; Jiang, L.; Guo, F.; Ren, S.; Yao, L.; Yang, J. Property inﬂuence and poisoning mechanism of
HgCl2 on V2O5-WO3/TiO2 SCR-DeNOx catalysts. Catal. Commun. 2016, 85, 34–38. [CrossRef] 17. Klimczak, M.; Kern, P.; Heinzelmann, T.; Lucas, M.; Claus, P. High-throughput study of the eﬀects of
inorganic additives and poisons on NH3-SCR catalysts—Part I: V2O5–WO3/TiO2 catalysts. Appl. Catal. B Environ. 2010, 95, 39–47. [CrossRef] 18. Chen, J.P.; Buzanowski, M.A.; Yang, R.T.; Cichanowicz, J.E. Deactivation of the vanadia catalyst in the selective catalytic reduction process. J. Air Waste Manage. Assoc. 1990, 40, 1403–1409. [CrossRef] 19. Tokarz, M.; Järårs, S.; Persson, B. Poisoning of De-NOx SCR catalyst by ﬂue gases from a waste incineration plant. Stud. Surf. Sci. Catal. 1991, 68, 523–530.
20. Chen, L.; Li, J.; Ge, M. The poisoning eﬀect of alkali metals doping over nano V2O5–WO3/TiO2 catalysts on selective catalytic reduction of NOx by NH3. Chem. Eng. J. 2011, 170, 531–537. [CrossRef] 21. Song, L.; Zhang, R.; Zang, S.; He, H.; Su, Y.; Qiu, W.; Sun, X. Activity of selective catalytic reduction of NO
over V2O5/TiO2 catalysts preferentially exposed anatase  and  facets. Catal. Lett. 2017, 147, 934–945. [CrossRef] 22. Yu, W.; Wu, X.; Si, Z.; Weng, D. Inﬂuences of impregnation procedure on the SCR activity and alkali resistance
of V2O5–WO3/TiO2 catalyst. Appl. Surf. Sci. 2013, 283, 209–214. [CrossRef] 23. Wang, S.; Guo, R.; Pan, W.; Li, M.; Sun, P.; Liu, S.; Liu, S.; Sun, X.; Liu, J. The deactivation mechanism of
Pb on the Ce/TiO2 catalyst for the selective catalytic reduction of NOx with NH3: TPD and DRIFT studies. Phys. Chem. Chem. Phys. 2017, 19, 5333–5342. [CrossRef][PubMed] 24. Cao, J.; Yao, X.; Yang, F.; Chen, L.; Fu, M.; Tang, C.; Dong, L. Improving the denitration performance and 4+ 4+ K-poisoning resistance of the V2O5-WO3/TiO2 catalyst by Ce and Zr co-doping. Chin. J. Catal. 2019, 40, 95–104. [CrossRef]
25. Zhang, S.; Zhong, Q. Surface characterization studies on the interaction of V2O5–WO3/TiO2 catalyst for low temperature SCR of NO with NH3. J. Solid State Chem. 2015, 221, 49–56. [CrossRef] 26. Shi, Y.; Shu, H.; Zhang, Y.; Fan, H.; Zhang, Y.; Yang, L. Formation and decomposition of NH4HSO4 during selective catalytic reduction of NO with NH3 over V2O5-WO3/TiO2 catalysts. Fuel Process. Technol. 2016, 150, 141–147. [CrossRef] 27. Peng, Y.; Si, W.; Li, X.; Chen, J.; Li, J.; Crittenden, J.; Hao, J. Investigation of the poisoning mechanism of lead
on the CeO2-WO3 catalyst for the NH3-SCR reaction via in situ IR and Raman spectroscopy measurement. Environ. Sci. Technol. 2016, 50, 9576–9582. [CrossRef]
28. Gan, L.; Chen, J.; Peng, Y.; Yu, J.; Tran, T.; Li, K.; Wang, D.; Xu, G.; Li, J. NOx removal over V2O5/WO3–TiO2 prepared by a grinding method: Inﬂuence of the precursor on vanadium dispersion. Ind. Eng. Chem. Res. 2017, 57, 150–157. [CrossRef] 29. Li, X.; Li, K.; Peng, Y.; Li, X.; Zhang, Y.; Wang, D.; Chen, J.; Li, J. Interaction of phosphorus with a FeTiOx catalyst for selective catalytic reduction of NOx with NH3: Inﬂuence on surface acidity and SCR mechanism. Chem. Eng. J. 2018, 347, 173–183. [CrossRef] 30. Shao, G.; Wang, F.; Ren, T.; Liu, Y.; Yuan, Z. Hierarchical mesoporous phosphorus and nitrogen doped titania materials: Synthesis, characterization and visible-light photocatalytic activity. Appl. Catal. B Environ. 2009, 92, 61–67. [CrossRef] 31. Hiroyuki, K.; Katsumi, T.; Odenbrand, C.U.I. Surface acid property and its relation to SCR activity of
phosphorus added to commercial V2O5(WO3)/TiO2 catalyst. Catal. Lett. 1998, 53, 65–71. 32. Dong, Y.; Qu, R.; Hao, S.; Zheng, C.; Cen, K. Investigation of the promotion eﬀect of WO3 on the decomposition and reactivity of NH4HSO4 with NO on V2O5-WO3/TiO2 SCR catalysts. RSC Adv. 2016, 6, 55584–55592. 33. Parvulescu, V.I.; Boghosian, S.; Parvulescu, V.; Jung, S.M.; Grange, P. Selective catalytic reduction of NO with
NH3 over mesoporous V2O5–TiO2–SiO2 catalysts. J. Catal. 2003, 217, 172–185. [CrossRef] Catalysts 2020, 10, 345 14 of 14
34. Chen, L.; Li, J.; Ge, M. Promotional eﬀect of Ce-doped V2O5-WO3/TiO2 with low vanadium loadings for selective catalytic reduction of NOx by NH3. J. Phys. Chem. C 2009, 113, 21177–21184. [CrossRef] 35. Jiang, B.Q.; Wu, Z.B.; Liu, Y.; Lee, S.C.; Ho, W.K. DRIFT study of the SO2 eﬀect on low-temperature SCR reaction over Fe-Mn/TiO2. J. Phys. Chem. C 2010, 114, 4961–4965. [CrossRef] 36. Nova, I.; Lietti, L.; Tronconi, E.; Forzatti, P. Dynamics of SCR reaction over a TiO2-supported vanadia–tungsta commercial catalyst. Catal. Today 2000, 60, 73–82. [CrossRef] 37. Guo, R.; Wang, Q.; Pan, W.; Chen, Q.; Ding, H.; Yin, X.; Yang, N.; Lu, C.; Wang, S.; Yuan, Y. The poisoning
eﬀect of heavy metals doping on Mn/TiO2 catalyst for selective catalytic reduction of NO with NH3. J. Mol. Catal. A Chem. 2015, 407, 1–7. [CrossRef] + 38. Chang, H.Z.; Shi, C.N.; Li, M.G.; Zhang, T.; Wang, C.Z.; Jiang, L.L.; Wang, X.Y. The eﬀect of cations (NH4 , Na+,K+, and Ca2+) on chemical deactivation of commercial SCR catalyst by bromides. Chin. J. Catal. 2018, 39, 710–717. [CrossRef]
39. Yin, X.; Han, H.; Gunji, I.; Endou, A.; Ammal, S.S.C.; Kubo, M.; Miyamoto, A. NH3 adsorption on the brönsted and lewis acid sites of V2O5 (010): A periodic density functional study. J. Phys. Chem. B 1999, 103, 4701–4706. [CrossRef]
40. Ye, J.; Gao, X.; Zhang, Y.; Wu, W.; Song, H.; Luo, Z.; Cen, K. Eﬀects of PbCl2 on selective catalytic reduction of NO with NH3 over vanadia-based catalysts. J. Hazard. Mater. 2014, 274, 270–278. 41. Yang, Y.; Xu, W.; Wu, Y.; Wang, J.; Zhu, T. Inhibition eﬀect of HBr over a commercial V2O5-WO3/TiO2 catalyst in a NH3-SCR process. Catal. Commun. 2017, 94, 82–85. [CrossRef] 42. Yang, J.; Yang, Q.; Sun, J.; Liu, Q.; Zhao, D.; Gao, W.; Liu, L. Eﬀects of mercury oxidation on V2O5–WO3/TiO2 catalyst properties in NH3-SCR process. Catal. Commun. 2015, 59, 78–82. [CrossRef] 43. Sheng, H.; Zhou, J.; Zhu, Y.; Luo, Z.; Ni, M.; Cen, K. Mercury oxidation over a Vanadia-based selective catalytic reduction catalyst. Energy Fuels 2009, 23, 253–259. 3- 31 44. Sudarsan, V.; Muthe, K.P.; Vyas, J.C.; Kulshreshtha, S.K. PO4 tetrahedra in SbPO4 and SbOPO4:A P NMR and XPS study. J. Alloys Compd. 2002, 336, 119–123. [CrossRef]
45. Jiang, H.; Wang, Q.; Zang, S.; Li, J.; Wang, Q. Enhanced photoactivity of Sm, N, P-tridoped anatase-TiO2 nano-photocatalyst for 4-chlorophenol degradation under sunlight irradiation. J. Hazard. Mater. 2013, 261, 44–54. [CrossRef][PubMed]
46. Lei, T.; Li, Q.; Chen, S.; Liu, Z.; Liu, Q. KCl-induced deactivation of V2O5-WO3/TiO2 catalyst during selective catalytic reduction of NO by NH3: Comparison of poisoning methods. Chem. Eng. J. 2016, 296, 1–10. [CrossRef]
47. Zhang, S.; Li, H.; Zhong, Q. Promotional eﬀect of F-doped V2O5–WO3/TiO2 catalyst for NH3-SCR of NO at low-temperature. Appl. Catal. A Gen. 2012, 435–436, 156–162. [CrossRef]
48. Li, Q.; Chen, S.; Liu, Z.; Liu, Q. Combined eﬀect of KCl and SO2 on the selective catalytic reduction of NO by NH3 over V2O5/TiO2 catalyst. Appl. Catal. B Environ. 2015, 164, 475–482. [CrossRef] 49. You, Y.; Shi, C.; Chang, H.; Guo, L.; Xu, L.; Li, J. The promoting eﬀects of amorphous CePO4 species on phosphorus-doped CeO2/TiO2 catalysts for selective catalytic reduction of NOx by NH3. Mol. Catal. 2018, 453, 47–54. [CrossRef] 50. van Der Bij, H.E.; Weckhuysen, B.M. Phosphorus promotion and poisoning in zeolite-based materials: Synthesis, characterisation and catalysis. Chem. Soc. Rev. 2015, 44, 7406–7428. [CrossRef]
51. Yang, S.; Wang, C.; Ma, L.; Peng, Y.; Qu, Z.; Yan, N.; Chen, J.; Chang, H.; Li, J. Substitution of WO3 in V2O5/WO3–TiO2 by Fe2O3 for selective catalytic reduction of NO with NH3. Catal. Sci. Technol. 2013, 3, 161–168. [CrossRef] 52. Szaleniec, M.; Drzewiecka-Matuszek, A.; Witko, M.; Hejduk, P. Ammonium adsorption on Brønsted acidic centers on low-index vanadium pentoxide surfaces. J. Mol. Model. 2013, 19, 4487–4501. [CrossRef][PubMed]
53. Shen, B.; Wang, F.; Zhao, B.; Li, Y.; Wang, Y. The behaviors of V2O5–WO3/TiO2 loaded on ceramic surfaces for NH3–SCR. J. Ind. Eng. Chem. 2016, 33, 262–269. [CrossRef]
© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).